Pré-visualização3 páginas

Acta Metallurgica Slovaca, Vol. 16, 2010, No. 2, p. 76-83 76 OPTIMIZATION OF TUNDISH EQUIPMENT B. Buľko, J. Kijac Department of Ferrous Metallurgy and Foundry, Faculty of Metallurgy, Technical University Košice, Slovakia Received 08.06.2010 Accepted 26.06.2010 Corresponding author: B. Buľko, Tel: +21 55 602 3153, E-mail: branislav.bulko@tuke.sk, Department of Ferrous Metallurgy and Foundry, Faculty of Metallurgy, Technical University Košice, Slovakia Abstract This paper compares residence times of non equipped tundish and tundish equipped with Turbostop and weirs at three different casting speed. Set of measurements in this paper was performed in laboratory simulated flow processes (LSSP). Water model is assembled at scale 1:3 to original. Measurements were evaluated by graphical measuring of water conductivity variation at tundish inlet and outlet by adding potassium chloride into tundish inlet and visually where KMnO4 was used as indicator. Within the frame of tundish equipment optimization three different variants were compared with support of Turbostop and weirs in two different distances from impact area. Keywords: tundish, continuous casting, water model, physical modelling Introduction In present 92,8% of world steel production is casted on continuous casting machine [1]. Therefore great emphasis is given to maximalize effectivity of this process. The key phase of continuous casting is tundish so that’s why major attention is given to it [2]. Beside of refining effect of slag phase also steel flow in tundish is very important factor [3]. Study of liquid metal flow in tundish in continuous casting of steel is problematic in practical conditions in term of great count of empirical experiments or technological difficulty of performing these experiments, they are also expensive. In term of mentioned problems physical or mathematical modelling is used for simulation, eventually combination of these methods [4-5]. In physical modelling is molten steel substituted by water, which also allows visual flow examination in tundish [6-7]. This substitution of flow medium is made by similar viscosity parameters for water and steel Tab.1 [8]. Table 1 Comparison of physical properties of water at 20°C and steel at 1600°C (1) Property Water at 20°C Steel at 1600°C Dynamic viscosity (kg.m-1.s-1) 0,001 0,0064 Density (kg.m-3) 1000 7014 Kinematic viscosity (m2.s-1) 1.10-6 0,913.10-6 Surface tension (N.m-1) 0,073 1,6 Flow of steel in tundish is affected by geometry of tundish, dimensions, shape and arrangement of dams and weirs, steel level in tundish, volume flowages, position of ladle shroud, there through quality of steel is expressively influenced [9-11]. Acta Metallurgica Slovaca, Vol. 16, 2010, No. 2, p. 76-83 77 Used methods Number of various measuring methods was developed by worldwide intensive long term study of possibilities of flow in tundish. [12]. Tundish can operate in two modes. Case that steel level in tundish is constant and amount of steel incoming into tundish is equivalent to steel amount leaving tundish through shrouds we call Steady State. If tundish operates in transient casting it means that steel flow in tundish is changing with time together with steel level in tundish. These happen during changing of ladles [13-14]. Noted experiments were performed in steady state. For discovering residence times of tundish was used LSPP water model for continuous casting in 1:3 scale. In this article so called C-curves method was used which allows us to define characteristics of steel flow in tundish at constant parameters of casting [15]. After reaching required level in crystallizer and establishing of cast speed water solution of KCl is injected into ladle shroud. Conductivity probes are placed on entry into tundish and its shrouds which records changes of conductivity of water effected by added salt by which C-curve is acquired [16-17]. By this curve we can determine minimum residence time τmin which is minimum time for injected fugitive dye into ladle shroud (τ0 =0s) detected at tundish shroud. Maximum residence time have definitive influence on time which inclusions have to rise from steel into slag [18-20]. Maximum residence time τmax is time between τ0 and maximum measured concentration of fugitive dye on shroud [21-22]. Non equipped tundish was compared with tundish equipped with Turbostop [23], Turbostop and weirs in distance 480mm or 570mm from center at three various casting speed Fig.1. There are 12 measurements presented in the paper. Water model consists of two ladles which are able to change during simulation of casting, ladle shroud and tundish which outlet through shrouds into crystallizers are regulated by two stopper rod. Induction flow meters are placed in every separate shroud. Every vessel has temperature and level meter. Model is controlled by electronic system Simatic, which can control every flow rate, levels, ladle shift and ladle shroud. Water can be supplied externally or can circulate in model. Model is equipped with instruments for temperature and conductivity reading from Moravian Instruments concern. Water heating system is installed for non-isothermic measurements. Fig.1 Used flow modificator combinations in tundish KCl was injected to the ladle shroud together with KMnO4, which acted as contrastive substance, what also enabled visual observation of flow in the tundish. Measured conductivity values were converted to dimensionless concentration owing to uniform form of obtained curves. Acta Metallurgica Slovaca, Vol. 16, 2010, No. 2, p. 76-83 78 Conditions of similarity In the case of utilization of longitudinal criterion of 1:1, the model would meet the Reynolds and Froud criterions of similarity. Because of reasons mentioned above the model was constructed in the scale 1:3, and so based on its dimensions gravity and inertial forces were abided. For this reason it was not simultaneously possible to abide gravity and viscosity similarity requirements. Gravity and inertial forces are characterized by Froud criterion for model as well as for original [24]: ´FrFr = (1) ´´. ´ . 22 lg w lg w = (2) Where: w is speed [m.s-1] g is acceleration of gravity [m.s-2] l is length [m] Both this original and model are exposed to the same gravity acceleration and that’s why this can by neglected, thus next equation is obtained: ´ ´ 22 l w l w = (3) Time is then established by the ratio: w l =τ Where: τ is time [s] (4) Next relationships are acquired by gradual derivation [6]: 2 τMM l = (5) 5 2 Ql MM = (6) Where: M1 is longitudinal scale, Mτ is time scale MQ is scale of volume flow In the case of model constructed in the scale 1:3 the M1 is 0,33. For the original with mold dimensions of 225x1590 mm we can consider at casting velocity with minute production Qm = 5335kg/min, if we consider steel density ς=7800kg.m-3. Volume flow rate from ladle to the tundish is then Qv=0,0475m3.min-1=47,58l.min-1. If this volume flow rate is abided in the model, then Fr=Fr´ condition is satisfied. According to the equation (5), the time scale is then: 5773,033,0 2 1 2 1 === lMM τ (7) From the mentioned calculations it results that within the used water model there will be reached velocities 1,73 times lower than on the work and at satisfying equation (1) there will be similar states reached at time 1,73 times shorter that on the original [6]. Acta Metallurgica Slovaca, Vol. 16, 2010, No. 2, p. 76-83